Fabrication of tin-filled carbon nanofibres by microwave plasma vapour deposition and their in situ heating observation by environmental transmission electron microscopy
© Tokunaga et al.; licensee Springer. 2013
Received: 8 April 2013
Accepted: 16 June 2013
Published: 28 June 2013
Sn-filled carbon nanofibres (CNFs) are fabricated by microwave plasma chemical deposition. Scanning electron microscopy observations revealed the existence of a Sn island under the CNFs. The structure of the CNFs is investigated, and the behaviour of Sn in the internal space of CNFs is revealed by performing in situ heating observations by environmental transmission electron microscopy (ETEM). ETEM observations reveal that they have low-crystallized carbon wall and Sn occupies not only the CNF’s internal space but also its carbon wall. The Sn inside the CNF is completely covered by the carbon wall. Further, the in situ heating observations reveal that Sn within the internal space and the carbon wall of the CNFs diffused to the outside during heating. Moreover, it is found that higher membered carbon rings and defects in the graphite layer act as diffusion routes between disordered carbon layers.
Several methods for growing functionalized carbon nanotubes (CNTs) and carbon nanofibres (CNFs) have been proposed [1–4]. Further, methods for using the internal space of CNTs and CNFs have also been proposed. Some groups investigated methods for filling this internal space with metals during CNT and CNF growth [5–7]. Metal-filled CNFs (MFCNFs) are well-known carbon nanomaterials that can be easily fabricated by microwave plasma-enhanced chemical vapour deposition (MPCVD) with catalysts. During MPCVD, metal catalysts used in the fabrication of MFCNFs are introduced inside the MFCNFs. Various metals have been introduced into the internal space of MFCNFs, and the physical properties of these metals within the MFCNFs have been studied [5, 8, 9]. However, the behaviour of such metals inside CNFs and CNTs, especially under heating, has not been widely studied. In the present study, Sn-filled CNFs were fabricated by MPCVD and characterized by environmental transmission electron microscopy (ETEM). Moreover, in situ heating observations by ETEM were carried out to reveal the behaviour of Sn within the CNFs under heating.
The Sn-filled CNFs were fabricated as follows: First, a thin Sn layer was fabricated on the surface of a 20 mm × 20 mm Si substrate with a natural oxide layer using a heating evaporation system. The evaporated substrate was transferred into an MPCVD chamber in air. The chamber was then evacuated to a pressure of 1 × 10−5 Pa. Next, hydrogen gas was introduced into the MPCVD chamber, and any remaining gas was purged from the chamber. The chamber pressure was kept at 20 Torr by introducing hydrogen gas at a flow rate of 50 sccm. The substrate was heated to 500°C and held at that temperature for 10 min under the hydrogen gas flow. Methane at 50 sccm and hydrogen at 50 sccm were introduced. The microwave plasma was then ignited, and a negative bias of 400 V was applied to the substrate, after which Sn-filled CNF growth began and continued for 10 min. The following conditions were maintained during the growth of the CNFs: a substrate temperature of 500°C, chamber pressure of 20 Torr, and microwave power of 700 W. After CNF growth, the microwave power was turned off, and the substrate temperature was gradually reduced under the hydrogen gas flow. When the substrate temperature reached approximately room temperature, the chamber pressure was brought up to atmospheric pressure by the introduction of nitrogen gas. Finally, the substrate was removed from the chamber. A commercial MPCVD system (Model AX5200, ASTeX, Cornes Technologies Limited, Minato-ku, Japan) was used for the fabrication of CNFs.
The Sn-filled CNFs grown on the Si substrate were characterized by ETEM (JEM-1000KRS, JEOL, Akishima-shi, Japan). They were collected from the substrate and deposited onto a metal grid thin foil with a carbon membrane using tweezers. The thin foil was then placed on a heated holder having a single-axis tilt mechanism (JEOL). The sample heating temperature was measured during the heating stage of the holder using a thermocouple placed directly in contact with the sample. The holder was inserted into the ETEM chamber, in which structural characterization, elemental analysis, and in situ heating observation by ETEM with electron energy loss spectroscopy (EELS) were performed. The sample heating temperature during the in situ observations was 400°C.
Results and discussion
Although many articles have reported the growth of metal-filled CNFs [12, 15–17], the present study describes the first successful growth of Sn-filled CNFs on a Si substrate by MPCVD. Moreover, our results reveal the existence of Sn not only in the internal spaces of the Sn-filled CNFs but also in their carbon walls. The metal filling mechanism in the internal spaces of the CNFs was considered almost the same as that reported by Hayashi et al., in which metal is introduced to the internal space by a capillary effect during CNF growth . Here, we discuss the reasons for the existence of Sn in the carbon wall. When the substrate was annealed, the Sn on the substrate formed particles. The plasma was then ignited, and the growth process began. The ions in the plasma collided with the surfaces of the Sn particles. Although these collisions increase the surface temperature of the particles, the exact temperature of the Sn particles was not determined. However, the surface temperature of the Sn particles is believed to have been approximately the same as the plasma temperature (several thousands of degrees Celsius ) because the substrate was covered completely by the plasma. The introduction of Sn into the carbon walls of the CNFs under these conditions could be explained by various phenomena. The first possibility is that Sn directly introduced into the carbon wall from under the CNF during the carbon wall owing to the solution of infinitesimal amounts of Sn in the carbon. However, the solid solution quantity of Sn in C is 0.002 at .% at several thousands of degrees Celsius . The solution of Sn into the carbon wall could have dislocated the carbon wall during its formation, resulting in defects in the carbon wall. The second possibility is the diffusion of Sn present at the bottom of CNF as well as within the CNFs into the carbon wall. This diffusion of Sn could have occurred during plasma and substrate heating in the CNF growth process. The diffused Sn is considered to have remained in the carbon wall. The diffusion route of Sn in the carbon wall has been discussed in the paragraph describing the in situ heating observations. The third possibility is that Sn ions collided into the carbon wall. As mentioned above, the surface temperature of Sn particles on the substrate during MPCVD was extremely high. Previously reported MFCNFs had Fe, Co, Ni, or Cu only in their internal spaces [12, 15–17], and these metals have high boiling points of 2,750°C, 2,900°C, 2,730°C, and 2,595°C , respectively. In contrast, the boiling point of Sn is about 2,270°C, which is lower than those of Fe, Co, Ni, and Cu. These values indicate that compared to these other metals, Sn is easier to evaporate at around the plasma temperature. This suggests that the Sn supplied in the plasma by Sn evaporation was ionized in the plasma, and the ionized Sn was attracted to the substrate by the negative bias, colliding with the CNFs growing on the substrate. The Sn was then deionized and remained in the carbon wall. When the ionized Sn collided with the CNFs, the fine carbon wall construction was possibly disturbed, damaging the carbon wall. There is also a possibility that Sn that was present on the substrate and sputtered by the bias-enhanced plasma collided with the CNFs. Sputtered metal typically exists as clusters in which some atoms aggregate. If clusters existed on and/or in the CNFs’ carbon walls, dark round contrasts would appear in TEM images. However, such dark contrasts do not appear in Figure 2a, so this possibility is low. These considerations leave us with the following three possibilities: Sn in the carbon wall was directly introduced to the carbon wall by the solution of Sn in carbon; Sn diffused into the carbon wall from beneath and within the CNF; and/or Sn on the substrate evaporated owing to heating by the plasma, and the evaporated Sn ionized in the plasma, collided with the CNFs, and diffused into the carbon wall.
These results clearly show that Sn can diffuse into the carbon wall of CNFs fabricated by MPCVD. The method of Sn diffusion into and out of the CNF is peculiar. It is certain that Sn diffused in the carbon wall because Sn was perfectly covered by the carbon wall (Figure 4). The carbon wall had a graphite structure (Figure 2b), and there are two possible routes for the Sn diffusion. One is the 0.33- to 0.34-nm gap between the graphite layers, and the other is a hole in the six-membered carbon ring, which is 0.14 nm on a side . The maximum diameter of a six-membered ring is 0.28 nm, which is narrower than the distance between graphite layers. Hence, we speculate that Sn atoms diffuse preferentially in the space between the graphite layers. However, the carbon walls of our CNFs contain defects (Figure 2b), and hence, they exhibit a disordered structure similar to disordered graphite layers, higher membered carbon rings (e.g. seven- and eight-membered rings), and disjointedness in graphite layers. These structures are believed to function as the new third route for the Sn diffusion. Ng et al. suggested these three routes for the diffusion of Li ion into the carbon wall. In carbon rings, Li ions diffused more easily owing to defects such as those in carbon rings with more than six members . In particular, carbon walls near the top of the CNFs have three-dimensionally curved walls such as those in fullerene, and hence, higher membered carbon rings exist at the top of the CNFs, leading to easy Sn diffusion there. As observed in Figure 4, Sn was eliminated from the top of the carbon wall of CNFs, which further suggests that Sn easily diffuses from the top of the CNFs. These in situ heating observation results provided us with remarkably important information that Sn can diffuse from within CNF carbon walls with defects to the outside of the CNF. This suggests that materials of approximately the same size or smaller than the Sn atoms can diffuse through a defective carbon wall.
It is expected that the Sn-filled CNFs fabricated by MPCVD in this study can be utilized for hydrogen storage. Metals used for hydrogen storage, such as Sn, are generally frazzled , and this shape is changed by hydrogen adsorption and desorption. This process degrades the hydrogen storage properties of the metals. In the Sn-filled CNFs fabricated in this study, Sn is covered by a carbon wall that may prevent Sn frazzling, thus helping Sn maintain its hydrogen storage properties. Thus, the Sn-filled CNFs can likely be used as a hydrogen storage material.
We carried out structural analysis and in situ heating observations of Sn-filled CNFs grown by MPCVD. Sn was found to exist in the internal spaces as well as the carbon walls of the CNFs. Three possible mechanisms for the introduction of Sn into the carbon wall were discussed. The first possibility is that Sn was introduced directly from the Sn particles on the substrate during CNF growth. The second is that Sn diffused from the Sn beneath and within the CNF. The third is that Sn evaporated into plasma by the high plasma temperature collided with the CNF wall and was introduced into the carbon wall by negative bias. Moreover, by observing the heating of Sn-filled CNFs, we confirmed that Sn in the internal space and in the carbon wall of the CNF diffused to the outside through the carbon wall. The Sn is considered to pass through the space between disordered carbon layers, higher membered carbon rings, and defects in the graphite layer.
This work was supported by a Grant-in-Aid for Young Scientists (B program, no. 22760537), the Advanced Characterization Nanotechnology Platform of the National Institute for Materials Science, and the High Voltage Electron Microscope Laboratory of Nagoya University.
- Yudasaka M, Kataura H, Ichihashi T, Qin CL, Kar S, Iijima S: Diameter enlargement of HiPco single-wall carbon nanotubes by heat treatment. Nano Lett 2001, 1: 487–489. 10.1021/nl010037xView ArticleGoogle Scholar
- Hata K, Futaba ND, Mizuno K, Namai T, Yumura M, Iijima S: Water-assisted highly efficient synthesis of impurity-free single-walled carbon nanotubes. Science 2004, 306: 1362–1364. 10.1126/science.1104962View ArticleGoogle Scholar
- Chhowalla M, Teo KBK, Ducati C, Pupesinghe , Amaratunga JAG, Ferrari CA, Roy D, Robertson J, Milne IW: Growth process conditions of vertically aligned carbon nanotubes using plasma enhanced chemical vapor deposition. J Appl Phys 2001, 90: 5308–5317. 10.1063/1.1410322View ArticleGoogle Scholar
- Alosfur F, Jumali HHM, Radiman S, Ridha JN, Yarmo AM, Umar AA: Visible light-responsive TiO2 coated MWCNTs as a hybrid nanocatalysts. Int J Electrochem Sci 2013, 8: 2977–2982.Google Scholar
- Muller C, Hampel S, Elefant D, Biedermann K, Leonhardt A, Ritschel M, Buchner B: Iron filled carbon nanotubes grown on substrates with thin metal layers and their magnetic properties. Carbon 2006, 44: 1746–1753. 10.1016/j.carbon.2005.12.036View ArticleGoogle Scholar
- Maniwa Y, Kataura H, Abe M, Suzuki S, Achiba Y, Kira H, Matsuda K: Phase transition in confined water inside carbon nanotubes. J Phys Soc Japan 2002, 71: 2863–2866. 10.1143/JPSJ.71.2863View ArticleGoogle Scholar
- Hayashi Y, Fujita T, Tokunaga T, Kaneko K, Butler T, Rupesinghe N, Carey DJ, Silva PRS, Amaratunga JAG: Encapsluation of Co and Pd multi-metal nanowires inside multiwalled carbon nanotubes by microwave plasma chemical vapor deposition. Diamond Relat Mater 2007, 16: 1200–1203. 10.1016/j.diamond.2006.11.039View ArticleGoogle Scholar
- Gao Y, Bando Y, Liu Z, Golberg D, Nakanishi H: Temperature measurement using a gallium-filled carbon nanotube nanothermometer. Appl Phys Lett 2003, 89: 2913–2915.View ArticleGoogle Scholar
- Nagata A, Sato H, Matsui Y, Kaneko T, Fujiwara Y: Magnetic properties of carbon nanotubes filled with ferromagnetic metals. Vacuum 2013, 87: 182–186.View ArticleGoogle Scholar
- Ci L, Xie S, Tang D, Yan X, Li Y, Liu Z, Zou X, Zhou W, Wang G: Controllable growth of single wall carbon nanotubes by pyrolizing acetylene on the floating iron catalysts. Chem Phys Lett 2001, 349: 191–195. 10.1016/S0009-2614(01)01098-3View ArticleGoogle Scholar
- Popovska N, Danova K, Jipa I, Zenneck U: Catalytic growth of carbon nanotubes on zeolite supported iron, ruthenium and iron/ruthenium nanoparticles by chemical vapor deposition in a fluidized bed reactor. Powder Tech 2011, 207: 17–25. 10.1016/j.powtec.2010.10.005View ArticleGoogle Scholar
- Tyagi KP, Singh KM, Misra A, Palnitkar U, Misra SD, Titus E, Ali N, Cabral G, Gracio J, Roy M, Kulshreshtha KS: Preparation of Ni-filled carbon nanotubes for key potential applications in nanotechnology. Thin Solid Films 2004, 469–470: 127–130.View ArticleGoogle Scholar
- Zou T, Li H, Zhao N, Shi C: Electromagnetic and microwave absorbing properties of multi-walled carbon nanotubes filled with Ni nanowire. J Alloy Comp 2010, 496: L22-L24. 10.1016/j.jallcom.2010.02.103View ArticleGoogle Scholar
- Ma X, Cai Y, Li X, Wen S: Growth and microstructure of Co-filled carbon nanotubes. Mat Sci and Eng A 2003, 357: 308–313. 10.1016/S0921-5093(03)00250-8View ArticleGoogle Scholar
- Kozhuharova R, Ritschel M, Elefant D, Graff A, Leonhardt A, Mönch I, Mühl T, Zotova GS, Schneider MC: Well-aligned Co-filled carbon nanotubes: preparation and magnetic properties. App Surf Sci 2004, 238: 355–359. 10.1016/j.apsusc.2004.05.237View ArticleGoogle Scholar
- Sengupta J, Jana A, Singh PDN, Jacob C: Effect of growth temperature on the CVD grown Fe filled multi-walled carbon nanotubes using a modified photoresist. Mate Res Bull 2010, 45: 1189–1193. 10.1016/j.materresbull.2010.05.017View ArticleGoogle Scholar
- Li H, Zhao N, He C, Shi C, Du X, Li J: Fabrication and growth mechanism of Ni-filled carbon nanotubes by the catalytic method. J Alloy Comp 2008, 465: 51–55. 10.1016/j.jallcom.2007.10.088View ArticleGoogle Scholar
- Lombardi G, Bénédic F, Mohasseb F, Hassouni K, Gicquel A: Determination of gas temperature and C2 absolute density in Ar/H2/CH4 microwave discharges used for nanocrystalline diamond deposition from the C2 Mulliken system. Plasma Sources Sci Technol 2004, 13: 375–386. 10.1088/0963-0252/13/3/003View ArticleGoogle Scholar
- Oden LL, Gokcen AN: Sn-C and Al-Sn-C phase diagrams and thermodynamic properties of C in the alloys: 1550°C to 2300°C. Metall Trans B 1993, 24B: 53–58.View ArticleGoogle Scholar
- Lyman T: Metals Handbook. 8th edition. Russell Township: American Society for Metals; 1961.Google Scholar
- Kelly TB: Physics of Graphite. London: Applied Science; 1981.Google Scholar
- Ng MF, Zheng J, Wu P: Evaluation of Sn nanowire encapsulated carbon nanotube for a Li-ion battery anode by DFT calculations. J Phys Chem 2010, 114: 8542–8545.View ArticleGoogle Scholar
- Smith PD: Hydrogen in Metals. Chicago: The University of Chicago Press; 1947.Google Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.